- Email: [email protected]

Contents lists available at ScienceDirect

Journal of the Mechanics and Physics of Solids journal homepage: www.elsevier.com/locate/jmps

A theory of finite strain magneto-poromechanics B. Nedjar IMSIA, ENSTA ParisTech, CNRS, CEA, EDF, Université Paris-Saclay, 828 bd des Maréchaux, 91762 Palaiseau, France

a r t i c l e i n f o

abstract

Article history: Received 30 March 2015 Received in revised form 19 July 2015 Accepted 6 August 2015 Available online 8 August 2015

The main purpose of this paper is the multi-physics modeling of magnetically sensitive porous materials. We develop for this a magneto-poromechanics formulation suitable for the description of such a coupling. More specifically, we show how the current state of the art in the mathematical modeling of magneto-mechanics can easily be integrated within the unified framework of continuum thermodynamics of open media, which is crucial in setting the convenient forms of the state laws to fully characterize the behavior of porous materials. Moreover, due to the soft nature of these materials in general, the formulation is directly developed within the finite strain range. In a next step, a modeling example is proposed and detailed for the particular case of magneto-active foams with reversible deformations. In particular, due to their potentially high change in porosity, a nonlinear porosity law recently proposed is used to correctly describe the fluid flow through the interconnected pores when the solid skeleton is finitely strained causing fluid release or reabsorption. From the numerical point of view, the variational formulation together with an algorithmic design is described for an easy implementation within the context of the finite element method. Finally, a set of numerical simulations is presented to illustrate the effectiveness of the proposed framework. & 2015 Elsevier Ltd. All rights reserved.

Keywords: Magneto-poromechanics Continuum thermodynamics Biot's theory Large deformation Magneto-active foams

1. Introduction Magneto-active polymers (MAPs) are mostly composites of a soft polymer matrix impregnated with magnetically permeable particles, typically iron particles in micro- or nano-meter size. In general, the response of MAPs to magnetic fields can be divided into two categories based on the property of the matrix material: they can give large and prompt deformation, or they can change their mechanical properties with moderate straining. These two features have received considerable attention in recent years due to their potential applications including, for instance, sensors, actuators, and biomedicine, see for example Jolly et al. (1996), Zrínyi et al. (1996), Ginder et al. (2002), Varga et al. (2006) among many others. In parallel, the mathematical modeling of the coupling of electromagnetic fields in deformable materials has also been an area of active research. Fully coupled nonlinear field theories have been developed with constitutive formulations based on augmented free energy functions, see for instance Dorfmann and Ogden (2004a), Ericksen (2006), Kankanala and Triantafyllidis (2004), Steigmann (2004), Vu and Steinmann (2007). In particular, it has been shown that any one of the magnetic induction, magnetic field, or magnetization vectors can be used as an independent variable for the magnetic part of the problem, the other two being obtained through the constitutive relations. The relevant equations are based on the pioneering work of Pao (1978), see also Brown (1966), Kovetz (2000) for detailed discussions concerning these topics. This work is devoted to the modeling of the particular case of magneto-active foams. These latter have a combination of E-mail address: [email protected] http://dx.doi.org/10.1016/j.jmps.2015.08.003 0022-5096/& 2015 Elsevier Ltd. All rights reserved.

294

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

desirable properties, including high porosity, light weight, low cost and fast responsiveness to external stimuli. Indeed, they have the ability to respond to magnetic fields with drastic change in volume, shape, and porosity. Furthermore, when the porosity is highly interconnected, they can be good candidates for biomedical systems used to control drug delivery, see Liu et al. (2006), Zhao et al. (2011), or to dynamically control flows in microfluidic chips, see Hong et al. (2014). It becomes then of interest to develop a theory that couples the magnetic field with the large deformation in porous media. Historically, two approaches have been used in a relevant literature for the modeling of porous materials: mixture theories, see for example Bowen (1982), Wilmanski (2003), and the macroscale consolidation theory of Biot, see for example Biot (1941, 1972). The former approach is mostly used to model species migration where the mixture equations for mass balance are used in combination with classical equations for linear momentum balance in terms of rule-of-mixture relations for the stress response, see the recent examples of application in Duda et al. (2010), Baek and Pence (2011) among others. The present work is based on the latter approach, i.e. Biot's theory. Since the pioneering work of Biot, considerable progress has been made in the last decades to develop a concise framework in the domain of poromechanics. Briefly, it describes the evolution of a saturated porous material in terms of the deformation of its solid skeleton part on the one hand, and in terms of the distribution of the mass of its fluid part, on the other hand. The resulting boundary value problem consists of a coupling between the balance equation and the mass conservation of the fluid. The reader is referred for example to Lewis and Schrefler (1998), Coussy (2004) for a detailed synthesis. The coupling with magnetostatics is integrated within the framework of continuum thermodynamics of open media for the correct setting of the whole set of constitutive relations. In particular, to describe the potentially high change of porosity, we use a simplified version of the porosity law recently proposed in Nedjar (2013a), see also Nedjar (2013b). This law accounts for the physical property that the actual (Eulerian) porosity must belong to the interval [0, 1] for any admissible process as, by definition, the porosity is at any time a ratio of the connected porous space. Among others, this allows for a good description of the seepage process and the fluid release and/or absorption during the loading history. A further goal of this paper is the formulation of a finite element treatment to furnish a computational tool for structural simulations. The three-field boundary value problem at hand being strongly coupled, it must be solved with the help of a combination of existing numerical strategies proposed in a relevant literature. As a very first attempt, we opt for a monolithic scheme where the three sub-problems are solved simultaneously. The most relevant particularities of the proposed numerical scheme are highlighted for an easy implementation. An outline of the remainder of this paper is as follows. In Section 2, we recall the governing equations of mass conservation and mechanical balance together with the specialized versions of Maxwell's equations. Both of the equivalent spatial and material descriptions are considered. Then, in Section 3, the magneto-mechanics coupling is embedded within the framework of continuum thermodynamics. In particular, we show how the formulation can be based on the magnetic induction vector or, equivalently, on the magnetic field vector. Section 4 is devoted to the modeling of hyperelastic magnetoactive foams. Details of the whole constitutive equations are given together with the variational forms in view of the numerical approximation. This model example is then used for the simulations of Section 5. Finally, conclusions and perspectives are drawn in Section 6. Notation: Throughout the paper, bold face characters refer to second- or fourth-order tensorial quantities. In particular, 1 denotes the second-order identity tensor with components δij (δij being the Kronecker delta), and I is the fourth-order unit 1 tensor of components Iijkl = 2 (δ ik δjl + δ il δjk ) . The notation (·)T is used for the transpose operator and the double dot symbol ‘:’ is used for double tensor contraction, i.e. for any second-order tensors A and B , A: B = tr [ABT ] = Aij Bij where, unless specified, summation on repeated indices is always assumed. One has the property tr [(·)] = (·) : 1 for the trace operator “tr ”. The notation ⊗stands for the tensorial product. In components, one has (A ⊗ B )ijkl = Aij Bkl , and for any two vectors and , ( ⊗ )ij = Ui Vj . Furthermore, the double-striked characters will exclusively be used for vector fields related to the magnetic part of the problem, e.g. , , ….

2. Mass conservation and balance equations When undeformed, unstressed, and in the absence of magnetic fields, the magnetically sensitive porous body occupies the reference configuration Ω0 with boundary ∂Ω0 . The porous body is thought as being a superimposition of a solid skeleton and a fluid phase. By solid skeleton, we mean the continuum formed from the constitutive matrix and the connected porous space emptied of fluid. Its deformation is the one that is observable under the combined action of mechanical forces and magnetic fields. We identify a material solid skeleton particle by its position vector in the reference configuration, X ∈ Ω0 , and trace its motion by its current position at time t, x (X , t ) ∈ Ωt . The deformation gradient is as usual defined as F = ∇X x , where ∇X (·) is the material gradient operator with respect to the reference coordinates X . The Jacobian of the transformation is given by the determinant J = det F with the standard convention J > 0. Furthermore, for the porous space, we denote by n the Eulerian porosity which is the volume fraction of the connected porous space in the spatial configuration. Thus, for a current elementary volume dΩt of porous material, the volume of porous space within it is n dΩt . Now in contrast to the Eulerian porosity, the change in the porous space is thermodynamically better captured relative to the reference configuration through the Lagrangian porosity that we denote here by ϕ. This latter is defined by the following

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

295

Piola transform: If dΩ0 is the reference elementary volume to which dΩt corresponds, the relation ϕdΩ0 = ndΩt holds. Hence, as the relation between the elementary reference and current volumes is given by dΩt = J dΩ0 , we thereby get the important relation between the Lagrangian and Eulerian porosities

ϕ = Jn

(1)

2.1. Mass conservation for open systems Within a spatial elementary volume dΩt , the current fluid mass content is ρf n dΩt , where ρf is the actual fluid density. Likewise, the current solid mass content is ρs (1 − n) dΩt , where ρs is the actual density of the matrix that constitutes the solid skeleton. Therefore, by distinguishing the material time derivative with respect to the solid phase ds (·) /dt from the one relative to the fluid phase d f (·) /dt , the Eulerian forms of the mass conservations for the solid and fluid phases are respectively given by

ds dt

∫Ω

t

ρs (1 − n) dΩt = 0

and

df dt

∫Ω

t

ρf n dΩt = 0

(2)

for any partial or total volume Ωt of porous material. Furthermore, the fluid mass conservation (2)2 rewritten in terms of the material time derivative with respect to the solid phase is equivalently given by (see Appendix A for details),

ds dt

∫Ω

t

ρf n dΩt = −

∫Ω

t

div qf dΩt

(3)

where qf is the spatial flow vector of fluid mass, and given by

qf = ρf ν

with ν = n (vf − vs )

(4)

for the filtration vector ν , and the relative velocity (vf − vs ) of the fluid with respect to the velocity of the solid skeleton vs , see the sketch of Fig. 1 for an illustration. In Eq. (3), div(·) is the divergence operator with respect to the spatial coordinates x . It is denoted by Div(·) in the material configuration with respect to X . Furthermore, relative to the reference configuration, we introduce the Lagrangian fluid mass content, denoted here by Mf, and defined per unit of reference volume dΩ0 . It is related to the current fluid mass content per unit of current volume dΩt as Mf dΩ0 = ρf n dΩt . On the one hand, one obtains the well-known definition

Mf = ρf ϕ

(5)

where use has been made of the relation (1), and on the other hand, the spatial fluid mass conservation (3) leads to the following local Lagrangian form:

Ṁ f = − Div Q f

(6) JF −1qf .

where Q f is the material flow vector of fluid mass related to its spatial counterpart qf via the Piola transform Q f = In Eq. (6) and henceforth, the dot operator (·)̇ is the material time derivative with respect to the solid phase which reduces to a simple derivative with respect to time for a Lagrangian quantity. 2.2. Magnetostatics equations As the porous materials we consider are electrically non-conducting, the magnetostatic fields are governed by the following specializations of Maxwell's equations in the absence of distributed currents and time dependence:

Fig. 1. A magneto-active porous solid under a deformation φt of the solid skeleton and a fluid flow characterized by the flow vector qf .

296

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

̀ ′s law: curl = 0 in Ωt Ampere Gauss′s law: div = 0

in Ωt

(7)

where and are respectively the magnetic field and magnetic induction vectors, both with respect to the spatial configuration. They are related by the standard relation

= μ 0 ( + )

(8)

where is the spatial magnetization vector. The constant μ0 is the magnetic permeability of vacuum. In Eq. (7)1, curl(·) denotes the rotational operator with respect to x . It is denoted by Curl(·) in the material configuration with respect to X . Pull-back to the reference configuration gives the Lagrangian counterparts of the above laws:

Curl = 0 and

Div = 0

in Ω0

(9)

for the Piola transforms

= F T = JF −1 = F T

(10)

Using the relation (8), the Lagrangian magnetic induction vector given by Eq. (10)2 becomes

= μ 0 JC −1 ( + )

(11)

where C = FT F is the right Cauchy–Green tensor which, otherwise, is a strain measure for the solid skeleton. 2.3. Mechanical balance and power of external forces The magneto-active porous materials we have in mind are those where only the solid skeleton is sensitive to external magnetic fields. This fact is here taken into account within the classical Biot's theory. In statics, the spatial forms of the partial balance equations are given by s div ((1 − n) σs ) + m + ρs (1 − n) f + f int = 0 in Ωt ,

(1 − n) σs n = ts

on ∂Ωt

(12)

for the solid skeleton, and f div (nσ f ) + ρf nf + fint = 0 in Ωt ,

nσ f n = t f

on ∂Ωt

(13)

for the fluid phase. In these equations, σs and σf are respectively the partial Cauchy stress tensors relative to the solid skeleton and to the fluid phase, ts and t f are the respective prescribed Cauchy traction vectors on the boundary ∂Ωt of unit outer normal n , f is f s and fint are macroscopic interaction forces exerted by the other continuum. These latter the volumetric body force, and f int f s are such that f int + fint = 0 . And last, m is the magnetic body force per unit volume that solely affects the solid skeleton's partial mechanical balance. It is given by m = [∇x ]T , see for example Pao (1978). Here and in all what follows, the notation ∇x (·) refers to the spatial gradient operator with respect to the coordinates x . Adding up both contributions, we get the balance equation

div σ + m + ρf = 0 in Ωt

(14)

with

σ = (1 − n) σs + nσ f

and

ρ = (1 − n) ρs + nρf

(15)

for the total Cauchy stress tensor σ and the current density ρ of the porous material. Notice that due to the magnetization, the partial stress σs is in general non-symmetric, and so is the total stress σ . Nevertheless, we adopt here the well known structure where the stress is augmented with terms arising from the magnetic body force. Indeed, this latter can equivalently be written as, see for example Dorfmann and Ogden (2004a), Steigmann (2004), and Vu and Steinmann (2007), 1 m = div ( μ 0−1 ⎡⎣ ⊗ − 2 . 1⎤⎦ + . 1 − ⊗ ) =σm

(16)

where we have introduced for convenience the notation σm for the magnetic interaction stress tensor. The balance equation (14) can then equivalently be written as

div ∼ σ + ρf = 0 in Ωt

(17)

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

297

in terms of the augmented1 Cauchy stress tensor σ∼ defined by σ∼ = σ + σm . The stress σ∼ is this time symmetric. The pull-back of the balance equation (17) to the reference configuration gives the following useful Lagrangian form: ∼ Div P + ρ0 f = 0 in Ω0 (18)

∼ ∼ ∼ in terms of the augmented first Piola–Kirchhoff stress tensor P ≡ FS = Jσ∼F −T and the reference density ρ0 = Jρ , S being the augmented second Piola–Kirchhoff stress tensor. In particular, the first Piola–Kirchhoff magnetic interaction part Pm = Jσm F −T is

⎤ 1 ⎡ 1 ⎢ F ⊗ − C : ⊗ F −T ⎥ + . F −T − F −T ⊗ μ0 J ⎣ 2 ⎦

Pm =

(19)

where use has been made of the relations (10)2 and (10)3. For later use, let us compute the power of the external forces, 7ext , for the open system at hand. Adding up the contributions of both phases, it is given by

7ext =

∫Ω

t

s f (ρs (1 − n) f + m + f int ). vs + (ρf nf + fint ). vf dΩt

+

∫∂Ω

ts. vs + t f . vf da

(20)

t

Use of the divergence theorem after having replaced the boundary traction vectors (12)2 and (13)2, use of the relations (15), and simplifying with the balance equation (14), we get

∫Ω

7ext =

t

f σ: ∇x vs + f . qf + div (nσ fT (vf − vs )) + fint . (vf − vs ) dΩt

where the relation (4) for the spatial flow vector of fluid mass qf has been used. Furthermore, as the fluid partial stress tensor σf can be addressed through a spherical tensor, we henceforth adopt the form σf = − p1 for the fluid pore pressure p. f Finally, giving ride of the term fint . (vf − vs ) to the benefit of the fluid pore pressure, we end up with the form that will be used in the following thermodynamic developments:

7ext =

∫Ω

t

⎛p ⎞ σ: ∇x vs + f . qf − div ⎜⎜ qf ⎟⎟ dΩt ⎝ ρf ⎠

(21)

where the relation (4) has again been used. In Eq. (21), ∇x vs is the spatial velocity gradient of the solid skeleton that is related ̇ −1. to the deformation gradient through the well known kinematic relation ∇x vs = FF

3. Continuum thermodynamics and constitutive equations The above governing equations need now to be supplemented with adequate constitutive relations. These latter together with the characterization of the dissipation phenomena are constructed in accordance with the requirements of continuum thermodynamics. We demonstrate in this work how the current state of the art in magneto-mechanics can be embedded within the up to date poromechanics developments in a straightforward manner. 3.1. First principle: energy conservation With respect to the spatial configuration, the first law of thermodynamics for our magneto-sensitive open system is given by

ds dt

∫Ω

t

ρs (1 − n) es dΩt +

df dt

∫Ω

t

ρf nef dΩt = 7ext + 8 + 7m

(22)

where es and ef are the specific, i.e. per unit of mass, internal energies of the solid skeleton's constitutive matrix and the fluid phase, respectively. While the power of the external forces 7ext is given by Eq. (21), 8 is the thermal flux power and 7m is the magnetic power, respectively given by

8=

∫∂Ω

− q . n da t

and

7m =

∫Ω

− . t

ds d Ωt dt

(23)

1 Note that in the literature the widely used term is total stress, e.g. Bustamante et al. (2006). Here we prefer to use the term augmented stress instead. The term total is left to its classical meaning in poromechanics; the additional contributions of the solid skeleton and the fluid phase, i.e. the total stress σ defined in Eq. (15)1.

298

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

where q is the spatial heat flux vector. The left-hand side of Eq. (22) can be rewritten as

∫Ω

t

d se + e div vs + div (ef qf ) dΩt dt

(24)

where e = ρs (1 − n) es + ρf nef is the total volumetric internal energy of the porous material. With Eqs. (24), (21) and (23), the energy conservation (22) is rewritten as

∫Ω

t

d se + e div vs dΩt = dt

∫Ω

t

σ: ∇x vs − div (hf qf + q) + f . qf − .

ds d Ωt dt

(25)

where hf = ef + p/ρf is the specific enthalpy of the fluid, see Appendix B for useful details. Hence, the local form of the first law is given by

d se ds + e div vs = σ: ∇x vs − div (hf qf + q) + f . qf − . dt dt

(26)

which should be compared with the corresponding one for closed systems, see for example Pao (1978), Brigadnov and Dorfmann (2003). However, for the following developments, the Lagrangian form is better suited. The energy conservation (25) must then be pull-back to the reference configuration. Denoting by E the material total internal energy per unit reference volume of the solid skeleton such that E dΩ0 = e dΩt , we obtain the following correspondence for the left-hand side of Eq. (25):

∫Ω

t

d se ds + e div vs dΩt ≡ dt dt

∫Ω

e d Ωt = t

∫Ω

E ̇ dΩ 0

(27)

0

Likewise, for the terms on the right-hand side, we have

∫Ω

σ: ∇x vs dΩt = t

∫Ω

P : F ̇ dΩ 0

(28)

0

where P = JσF −T is the total first Piola–Kirchhoff stress tensor,

∫Ω

div q dΩt = t

∫Ω

Div Q dΩ0

(29)

0

where Q = JF −1q is the material heat flux vector, and so on for the other terms:

∫Ω

t

∫Ω

t

∫Ω

div (hf qf ) dΩt = f . qf dΩt = .

t

∫Ω

ds d Ωt = dt

0

∫Ω

0

Div (hf Q f ) dΩ0

f . FQ f dΩ0

∫Ω

− . F −T : F ̇ + F −T ⊗ : F ̇ + . ̇ dΩ0 0

(30)

where, for this latter, use has been made of the relations (10)2 and (10)3 together with the well known kinematic relation J ̇ = JF −T : F ̇ . Hence, the material counterpart of the local form (26) is then

E ̇ = P: F ̇ − Div (hf Q f ) − Div Q + f . FQ f + . F −T : F ̇ − F −T ⊗ : F ̇ − . ̇

(31)

where one can notice the presence of the three last terms related to the magnetic coupling. The former ones are classical in poromechanics, see e.g. Armero (1999), Coussy (2004). 3.2. Second principle and main dissipation inequality The second law of thermodynamics postulates the positiveness of the entropy production. It is written in the spatial configuration as

ds dt

∫Ω

t

ρs (1 − n) ss dΩt +

df dt

∫Ω

t

ρf nsf dΩt ≥ −

∫∂Ω

t

q. n da T

(32)

where ss and sf are the specific entropies of the skeleton's constitutive matrix and the fluid, respectively, and T is the absolute temperature. Denoting by S the total entropy per unit reference volume such that S dΩ0 = [ρs (1 − n) ss + ρf nsf ] dΩt , pull-back of the inequality (32) to the reference configuration using similar computations as those for the first principle, Section 3.1, we end

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

299

up with the local form

⎛ Q⎞ , = S ̇ + Div ⎜ sf Q f + ⎟ ≥ 0 ⎝ T⎠ for the rate of entropy production , . Now defining the volumetric free energy alone μf, respectively as

ψ = E − TS

and

(33)

ψ of the porous material as a whole, and the specific free enthalpy of the fluid

μf = hf − Tsf

(34)

we can write the total dissipation + = T , as

+ = + thr + + flw + + int ≥ 0

(35)

where

+ thr = −

1 Q . ∇X T T

(

+ flw = − Q f . ∇X μf + int

)

T

+ f . FQ f

= P: F ̇ + μf Ṁ f − ST ̇

+ . F −T : F ̇ − F −T ⊗ : F ̇ − . ̇ − ψ ̇

(36)

after combining Eqs. (31) and (33), and using the fluid mass conservation, Eq. (6). In Eq. (36)2, (∇X μf )T stands for the material gradient of μf taken at temperature T held constant. In the Clausius–Duhem inequality (35), we distinguish three forms of dissipation: + thr due to the heat conduction, +flw due to the seepage process, and the internal dissipation +int in the porous material. These three forms are common in thermo-poromechanics, except for the additional terms in (36)3 that arise from the contribution to the internal dissipation of the magnetic coupling. A Fourier-type law for the definition of the heat flux vector q (or Q ) is sufficient to satisfy + thr ≥ 0. Likewise, for the seepage process, Darcy's law furnishes an example for the definition of the flow vector of fluid mass qf (or Q f ) that satisfies +flw ≥ 0. Now following common arguments in continuum thermodynamics, the non-negative dissipation due to internal processes in the porous material is imposed separately, see e.g. Truesdell and Noll (1965), Germain et al. (1983). Its treatment is detailed in the next section.

3.3. Internal dissipation and constitutive equations In a first step, we rewrite the expression (36)3 in a more convenient form. For this, let ψsk and Ssk be the free energy and the entropy of the solid skeleton alone, both per unit reference volume, and respectively given by

ψsk = ψ − Mf ψf

and

Ssk = S − Mf sf

(37)

where ψf = μf − p/ρf is the specific free energy of the fluid, i.e. after combining (B.7) with (B.9) in Appendix B. That is, ψsk is obtained by extracting the volumetric free energy of the fluid from the total volumetric free energy ψ and, likewise, Ssk is obtained by extracting the volumetric entropy of the fluid from the total volumetric entropy S. Then, with the help of definition (5) for the fluid mass content and the state laws (B.10) for the fluid, the internal dissipation (36)3 takes the new form

+ int = P: F ̇ + p ϕ ̇ − Ssk T ̇ + . F −T : F ̇ − F −T ⊗ : F ̇ − . ̇ − ψsk ̇

(38)

where, among others, one can notice the conjugate character between the pore pressure p and the Lagrangian porosity ϕ, instead of the one between μf and Mf that appears in (36)3. However, in this form, ϕ is the independent variable for the fluid part and we wish to use p instead, i.e. we want ϕ as a function of p and not the reverse, see e.g. Biot (1972). For this, the free energy ψsk is partially inverted through the partial Legendre transformation

3 sk = ψsk − pϕ

(39)

and the internal dissipation becomes then

+ int = P: F ̇ − ϕ ṗ − Ssk T ̇ + . F −T : F ̇ − F −T ⊗ : F ̇ − . ̇ − 3̇ sk ≥ 0

(40)

with a free energy of the general form 3 sk ≡ 3 sk (F , , p, T ). Without loss of generality, material dissipations such as plasticity or viscoelasticity are not considered for the sake of clarity. Using the standard arguments of continuum thermodynamics, see for example Coleman and Gurtin (1967), Germain et al. (1983), we get the following state laws:

300

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

∂3 sk − . F −T + F −T ⊗ , ∂F ∂3 sk ∂3 sk and Ssk = − . ϕ= − ∂p ∂T

= −

P=

∂3 sk , ∂ (41)

To simplify further these constitutive equations, we introduce by similar arguments as in Dorfmann and Ogden (2004a,b) the augmented volumetric free energy Ωsk as 1

Ωsk (F , , p, T ) = 3 sk (F , , p, T ) + 2 μ 0−1J−1 C: ⊗

(42) ∼ With this latter, the augmented first Piola–Kirchhoff stress tensor P ≡ P + Pm is directly obtained by the simple form ∼ ∂Ωsk P = , ∂F

(43)

where use has been made of the definition (19) for Pm . Furthermore, the Lagrangian magnetic field vector is directly obtained as

=

∂Ωsk , ∂

(44)

after a combination with (41)2 and the magnetic relation (11). The forms for the Lagrangian porosity and entropy of the solid skeleton remain unchanged:

ϕ= −

∂Ωsk ∂p

and

Ssk = −

∂Ωsk . ∂T

(45)

In summary, given the augmented free energy function Ωsk, the results of the constitutive relations (43)–(45) are replaced into: the mechanical balance equation (18), or (17), the fluid mass conservation equation (6), Maxwell's magnetic equations (9), or (7), and the transient heat equation if any. Notice further that the internal dissipation, Eq. (40), can now be equivalently rewritten in a more compact form as

∼ + int = P : F ̇ − ϕ ṗ − Ssk T ̇ + . ̇ − Ω̇ sk ≥ 0

(46)

where, among others, the conjugate character between and replaces the one between and . 3.4. Formulation based on the magnetic field If instead of the magnetic induction vector , we wish to use the magnetic field vector as the main independent ⁎ magnetic variable, we define then the complementary version of Ωsk, denoted by Ωsk , through the following partial Legendre transformation: ⁎ Ωsk (F , , p, T ) = Ωsk (F , , p, T ) − .

(47)

so that, when replaced into the inequality (46), the following state laws are deduced: ⁎ ∼ ∂Ωsk P = , ∂F

= −

⁎ ∂Ωsk

∂

,

ϕ= −

⁎ ∂Ωsk

∂p

,

Ssk = −

⁎ ∂Ωsk

∂T

.

(48)

This very useful correspondence has been established by Bustamante et al. (2006) for a similar formulation developed for ⁎ closed systems. Now it remains to precise the general form of the function Ωsk in Eq. (47). For this, we use the complementary version χsk of the volumetric free energy 3 sk , Eq. (39), that depends this time on the magnetic field instead of the magnetic induction . It is given by 1

χsk (F , , p, T ) = 3 sk (F , , p, T ) + 2 μ 0 JC −1: ⊗ ,

(49)

see e.g. Kovetz (2000), Steigmann (2004), Bustamante et al. (2008) for a similar relation written in terms of the spatial magnetic vectors , and . Hence, after combining Eqs. (49) and (42) into Eq. (47), and using the magnetic relation (11), the following form is obtained: 1

⁎ Ωsk (F , , p, T ) = χsk (F , , p, T ) − 2 μ 0 JC −1: ⊗ .

(50) ⁎ Ωsk

In summary for a formulation based on the magnetic field vector, the augmented free energy function has the form (50) and is used for the constitutive relations given in (48). These latter are replaced as usual into the mechanical balance equation (18), or (17), the fluid mass conservation equation (6), Maxwell's magnetic equations (9), or (7), and the transient heat equation if any.

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

301

4. Modeling hyperelastic magneto-active foams Of interest for the developments presented below is the consideration of porous materials with fully reversible deformations. One can think to the example of macroporous ferrogels that change drastically their porosity and volume in response to the application of external magnetic fields, see for example Zhao et al. (2011), Hong et al. (2014). These materials are isotropic and, for the sake of simplicity, it is further assumed here that the temperature is constant. We choose to consider the magnetic field vector as the main independent magnetic quantity and we leave the magnetic induction ⁎ vector to be determined using a constitutive law. We therefore use the augmented free energy function Ωsk introduced earlier in Section 3.4. Now for objectivity reasons, the free energy function χsk in Eq. (50) must depend on the deformation gradient F only through the right Cauchy–Green tensor C , and for symmetry reasons, it depends on the magnetic field vector only through the tensor product ⊗ , i.e. χsk ≡ χsk (C , ⊗ , p). Then, use of the property ⁎ ∂Ωsk

∂F

= 2F

⁎ ∂Ωsk

∂C

gives the equivalent form for the state laws in (48): ⁎

∂Ω τ∼ ≡ J∼ σ = F 2 sk F T , ∂C

J = − F

⁎ ∂Ωsk

∂

,

ϕ ≡ Jn = −

⁎ ∂Ωsk

∂p (51)

∼ =S

where we have defined the augmented Kirchhoff stress tensor τ∼ . Furthermore, being an isotropic function of its arguments, χsk depends in the most general case on the collection of six irreducible invariants, see for example Spencer (1984), Holzapfel (2000), Steigmann (2004) for more details, 1

I2 = 2 (I12 − C: C ),

I1 = C: 1, I4 = . ,

I5 = C: ⊗

I3 = det C ≡ J 2 ,

and

I6 = C 2: ⊗ ,

(52)

where the first three ones are classical in isotropic hyperelasticity, and the latter three ones, the so-called pseudo-invariants, arise from the coupling with magnetics. To make matters as concrete as possible, the following augmented volumetric free energy that conforms with the general form (50) will be adopted in our modeling: 1

⁎ ′ (C ) + χ (J , p) + Ωsk = χsk + c3 c1 I4 + c2 I5 I6 − 2 μ 0 JC −1: ⊗ por poromechanics

magnetic coupling

(53)

augmentation

where c1, c2 and c3 are material parameters. The first two terms are related to the purely poromechanic part of the response, see for example Nedjar (2013a, 2014): χ′sk characterizes the drained response of the solid skeleton without the porous space contribution. It depends at most on the above three invariants I1, I2 and I3. The function χpor is the part that accounts for the action of the pore pressure on the solid skeleton through the internal walls of the porous space. Its dependence on the deformation gradient only through its Jacobian J is clear since, by essence, it is a volumetric phenomenon. Here and in all what follows, the prime notation (·)′ refers to effective drained quantities, and not a derivative with respect to any of their arguments. Hence, the augmented stress tensor of the second Piola–Kirchhoff type, Eq. (51)1, is given by

∼ S = S′ + S por + 2c2 ⊗ + 2c3 { ⊗ C + C ⊗ } 1

− 2 μ 0 J (C −1: ⊗ ) C −1 + μ 0 JC −1 ⊗ C −1

(54)

with, for the purely poromechanics part S = S′ + Spor

S′ = 2

′ ∂χsk ∂C

and

S por = JC −1

∂χpor ∂J

(55) 1

where, among others, use has been made of the well known kinematic formula ∂J /∂C = 2 JC −1. Equivalently for the Kirchhoff type stress tensor, we have

τ∼ = τ ′ + τpor + 2c2 b ⊗ b + 2c3 {b ⊗ b2 + b2 ⊗ b} −

1 μ J . 1 + μ 0 J ⊗ 2 0

(56)

where b = FFT is the (spatial) left Cauchy–Green tensor, and where we have used the relation (10)1 for . For the poromechanics part τ = τ ′ + τpor , we have

302

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

τ ′ = FS′F T ≡ 2

′ ∂χsk ∂b

b

and

τpor = J

∂χpor ∂J

1

(57)

where, for (57)1, use has been made of the well known result in isotropic elasticity since the three invariants of b are the same as the above ones I1, I2 and I3 for C , see e.g. Truesdell and Noll (1965), Chadwick (1976), Marsden and Hughes (1983). Furthermore, observe from (57)2 the spherical character of the Cauchy stress tensor σpor = J−1 τpor due to the presence of the internal fluid pore pressure. For the magnetic induction vector, we have from Eqs. (53) and 482,

c1 − 2c − 2c3 C 2 = − + μ 0 JC −1 2 C 2 (58)

= μ0 JC −1

or equivalently for the Kirchhoff-like spatial version, Eq. (51)2,

J = − c1b − 2 c2 b2 − 2c3 b3 + μ0 J 2 (59)

= μ0 J

which, when compared with the relations (11) and (8), respectively, one concludes that the parameters c1, c2 and c3 are in fact the magnetization parameters. For the porosity, the state law (48)3, or (51)3, gives

ϕ ≡ Jn = −

∂χpor ∂p

(60)

This latter will be particularly detailed in the following section. 4.1. Porosity law The magneto-active porous materials are in general characterized by a high porosity that can drastically change under the action of mechanical forces and/or magnetic fields. The porosity law must then be able to describe this fact, but always keeping in mind that the (true) Eulerian porosity n is by definition a volume fraction and, by consequence, is restricted to always belong to the interval [0, 1]. Among the laws proposed in Nedjar (2013a) that satisfy this restriction, we choose here the following simplified one:

⎡ p − p0 ⎤ n ≡ n (J , p) = 1 − (1 − h (J )) exp ⎢ − ⎥ ⎣ (1 − f0 ) Q ⎦

(61)

where p0 is the initial pore pressure, f0 is the initial connected porosity, Q is a Biot-like modulus, and the function h(J) is defined as

⎧ f Jm for J ≤ 1 ⎪ 0 ⎡ ⎤ h (J ) = ⎨ f m (J − 1) ⎥ for J ≥ 1 ⎪ 1 − (1 − f0 ) exp ⎢ − 0 ⎣ 1 − f0 ⎦ ⎩

(62)

where m > 0 is a material parameter. This latter function is no more than the drained porosity law since h (J ) ≡ n (J , p = p0 ).

Fig. 2. Porosity law n (J , p) . An illustration for J ≤ 1 and p ≥ p0 .

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

303

Observe further that, see Fig. 2 for an illustration:

For a high pore pressure, the actual porosity is limited by the upper physical bound, n → 1−. Under drained conditions with p = p0, the porosity strictly belongs to the interval [0, 1]. At the limiting case of an infinitesimal theory with J ≈ 1 + ε , where ε⪡1 is the infinitesimal volumetric strain, a first order development of the expression (61) near p = p0 gives the relation

n = f0 + f0 m ε +

p − p0 Q

which is the classical Biot's linear porosity law interpreting the above parameter Q as the initial Biot's modulus, and the product f0 m ≡ b as the so-called Biot's coefficient, e.g. see Biot (1941), Coussy (2004). The partial volumetric free energy function χpor (J , p) that leads to the porosity law (61) through the state law (60) and satisfies the requirements

χpor (J = 1, p = p0 ) = 0

and

∂χpor ∂J

(J , p = p0 ) = 0

is given by

⎡ p − p0 ⎤ ⎥ − 1) χpor = − J (p − p0 ) − J (1 − h (J )) Q (1 − f0 )(exp ⎢ − ⎣ Q (1 − f0 ) ⎦

(63)

With this latter, the stress part due to the action of the internal pore pressure on the solid skeleton is defined as well, i.e. Eq. (55)2 for Spor , or Eq. (57)2 for τpor . 4.2. Variational formulation of the coupled problem In magnetostatics, the magnetic field vector can be expressed as the gradient of some magnetic scalar potential that we denote here by φ, see for example Steigmann (2004) for more details. We write

= − ∇X φ

⇔

= − ∇x φ

(64)

so that Ampère's equation (7)1, or (9)1, is identically satisfied. It remains then to solve Gauss's equation (7)2, or (9)2. The balance equations consist then of a system involving the mechanical equilibrium, the magnetic Gauss's equation, and the fluid mass conservation. In a finite domain of the reference configuration Ω0, the weak form of the three-field coupled problem at hand is

∼ P : ∇X (δu) dΩ0 = Gext (δu)

∫Ω

0

∫Ω

0

∫Ω

0

. ∇X (δφ) dΩ0 =

∫∂Ω

Q dA 0

δp Ṁ f − Q f . ∇X (δp) dΩ0 = 0

(65)

which must hold for any admissible variations δu , δφ and δp , of displacement, magnetic potential and pore pressure, respectively. Eq. (65)1 is equivalent to the strong form (18) where Gext (δu ) is a short hand notation for the virtual work of external mechanical loading, assumed for simplicity to be deformation independent. Eq. (65)2 is the weak form of Gauss's equation (9)2 where Q = . N is the eventual nominal magnetic induction imposed on the boundary ∂Ω0 of unit normal N , or on part of it. Notice here that, for the sake of simplicity, the effect of the surrounding space is not considered regarding the magnetic field which normally must be satisfied everywhere, and not only inside the body. So that, Eq. (65)2 is in fact an approximation. Finally, Eq. (65)3 is equivalent to the strong form (6) with the pore pressure field p as primary variable. For simplicity, only Dirichlet-type boundary conditions are considered in the presentation for this latter. Darcy's law is used for the filtration vector ν , see Eq. (4), so that the spatial flow vector of fluid mass is defined as well:

ν = − k∇x p ⇒ qf = − ρf k∇x p

(66)

where the gravity effects are neglected. The parameter k > 0 is the spatial permeability coefficient of the isotropic porous medium and, by the Piola transform, the material flow vector Q f in Eq. (65)3 is then given by

Q f = − ρf JkC −1∇X p

(67) F −T ∇X (·),

where the useful relation ∇x (·) = for scalar fields, has been used. Last but not least, and irrespective of the solid skeleton, the actual density of the saturating fluid must be linked to the

304

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

pore pressure p by specifying a constitutive law. The fluid being considered here as barotropic, ρf ≡ ρf (p), we use the polytropic-like law proposed in Nedjar (2013a),

⎛ p ⎞g ρf (p) = ρ f0 ⎜ ⎟ ⎝ p0 ⎠

(68)

where ρ f0 is the initial fluid density, and g ∈ [0, 1] is a fluid parameter. This law encompasses both ideal gas and incompressible fluids as particular cases under isothermal conditions. In fact, one can immediately notice that:

for g¼0, the fluid is incompressible with ρf (p) = ρ f0, ∀ p. for g¼1, the constitutive law reduces to the one for ideal gas. 4.3. Outlines of the algorithmic approximation Different numerical strategies can be employed to solve this strongly coupled problem. One can think of a staggered scheme consisting of an initial solid phase at fixed magnetic potential and fluid content, followed by Gauss's equation and the fluid mass conservation, both at fixed deformation, see Nedjar (2014) for a similar development in poromechanics. However, as a first attempt, we choose here to use a high fidelity solution procedure by using a monolithic scheme where the three sub-problems are solved simultaneously via an iterative resolution procedure of the Newton– Raphson type. Nevertheless, each of these sub-problems needs to be linearized first. Below are the relevant points of this procedure. Mechanical balance equation Within a typical time interval [tn, tn + 1], the displacement u , the magnetic potential assumed to be known fields at time tn, i.e. {u n, φn , pn }. ∼ Now by noticing the identity P : ∇X (δu ) = τ∼: ∇x (δu ), Eq. (65)1 is then linearized as

∫Ω

φ, and the pore pressure field p are

∼ [∇x (Δu) τ∼. ∇x (δu) + ∇sx (δu): C: ∇sx (Δu)] dΩ0 0

+ + + + + +

∫Ω

0

∫Ω

0

∫Ω

0

∫Ω

0

∫Ω

0

∫Ω

s ∇xs (δu): ⎡⎣ −4c2 b∇x (Δφ) ⊗ b⎤⎦ dΩ0 s ∇xs (δu): ⎡⎣ −4c3 b∇x (Δφ) ⊗ b2⎤⎦ dΩ0 s ∇xs (δu): ⎡⎣ −4c3 b2∇x (Δφ) ⊗ b⎤⎦ dΩ0

∇xs (δu): [μ 0 J . ∇x (Δφ) 1] dΩ0 s ∇xs (δu): ⎡⎣ −2μ 0 J∇x (Δφ) ⊗ ⎤⎦ dΩ0

[∇xs (δu): 1J 0

= Gnext + 1 (δu ) −

∂σpor Δp] dΩ0 ∂p

∫Ω

∇xs (δu): τ∼ dΩ0 0

(69)

where Δu , Δφ and Δp are increments of displacement, magnetic potential, and pore pressure fields, respectively. The first integral on the left-hand side represents the classical term composed by the geometric and the material contributions to the ∼ linearization, C being the augmented spatial tangent modulus at fixed magnetic potential and pore pressure that is detailed in Appendix C. The last integral on the left-hand side represents the solid–fluid coupling term where we have introduced the notation σpor = ∂χpor /∂J for the volumetric Cauchy stress due to the pore pressure, see Eq. (57)2. All the intermediate integrals represent the magneto-mechanics coupling, and the right-hand side represents the residual of the mechanical part. The notation (·)s used in Eq. (69) stands for the symmetric part of a second-order tensor. In particular, ∇sx (·) is the symmetric gradient operator. We have omitted the subscripts n + 1 for the sake of clarity. Nevertheless, unless otherwise specified, all the variables are understood to be evaluated at the actual time tn + 1, i.e. b ≡ bn + 1, ≡ n + 1, n ≡ nn + 1 …. Gauss's magnetic equation: For Gauss's equation, by noticing the useful identities

∇X (δφ . ) = F . ∇x (δφ ) ≡ J . ∇x (δφ) ⎛ ∂Ω ⁎ ⎞ −⎜ sk ⎟ . (−δ ) ⎝ ∂ ⎠

the linearization of Eq. (65)2 is then given by

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

∫Ω

0

305

s ∇x (δφ). {−4c2 b∇sx (Δu) b − 8c3 ⎡⎣ b∇sx (Δu) b2⎤⎦ }

+ ∇x (δφ). {μ 0 J (∇sx (Δu): 1) − 2μ 0 J∇sx (Δu) } + ∇x (δφ). {2c1b + 2c2 b2 + 2c3 b 3 − μ 0 J1}∇x (Δφ) dΩ0 =

∫∂Ω

Q dA − 0

∫Ω

∇x (δφ). J dΩ0 0

(70)

where the first two terms on the left-hand side are related to the magneto-mechanics coupling, and the right-hand side is the residual of the magnetic Gauss's balance. Fluid mass conservation equation The fluid mass conservation (65)3 needs first to be discretized in time before linearization. For this, the rate form of the fluid mass content is detailed as

ṗ ∂n ∂n Ṁ f = gρf Jn + ρf nJ ̇ + ρf J J ̇ + ρf J ṗ p ∂J ∂p after combining the definitions (1) and (5), and using the fluid law, Eq. (68). Then, an implicit backward-Euler scheme applied to the evolution equation (65)3 gives the following time-discretized form:

∫Ω

δp 0

+ δp

⎡ p⎤ ⎡ J ⎤⎫ ρf J ⎧ n ⎨ g log ⎢ ⎥ + log ⎢ ⎥ ⎬ Δt ⎩ ⎣ pn ⎦ ⎣ Jn ⎦ ⎭ ⎪

⎪

⎪

⎪

⎫ ρf J ⎧ ∂n ∂n ⎨ (J − Jn ) + (p − pn ) ⎬ Δt ⎩ ∂J ∂p ⎭ ⎪

⎪

⎪

⎪

+ ρf J∇x (δp). k∇x p dΩ0 = 0

(71)

where use has been made of Darcy's law, Eq. (66)2, for the flow vector of fluid mass, and where Δt = tn + 1 − tn for the time interval. After lengthy, but straightforward algebraic manipulations and collecting terms, the linearization is given by

∫Ω

δp 0

⎛ ∂n ρf J ⎧ ⎪ ∂ 2n ⎞ ∂n ⎨ (J − Jn ) ⎜ +J 2⎟+J ⎪ ⎝ ∂J Δt ⎩ ∂J ⎠ ∂J

⎛ ⎞ ∂n ∂ 2n ⎟ + (p − pn ) ⎜⎜ +J +n ∂p∂J ⎟⎠ ⎝ ∂p ⎫ ⎛ ⎡ J⎤ ⎡ p ⎤⎞⎛ ∂n ⎞ ⎪ ⎜⎜ log ⎢ ⎥ + g log ⎢ ⎥ ⎟⎟ ⎜⎜ n + J ⎟⎟ ⎬ 1: ∇sx (Δu) ⎪ ∂J ⎠ ⎭ ⎣ Jn ⎦ ⎣ pn ⎦ ⎠ ⎝ ⎝ + ρf Jk {∇x (δp). ∇x p1 − 2∇x (δp) ⊗ ∇x p} : ∇sx (Δu) dΩ0 +

∫Ω

δp 0

⎛ g ∂n ρf J ⎧ ⎪ ∂ 2n ⎞ ⎨ (J − Jn ) ⎜ + ⎟ ⎪ ⎝ p ∂J Δt ⎩ ∂J ∂p ⎠

⎛ ⎞ g ∂n n ∂ 2n ⎟ ∂n + (p − pn ) ⎜⎜ + + +g p ∂p2 ⎟⎠ ∂p ⎝ p ∂p ⎫ ⎛ ⎡ J⎤ ⎡ p ⎤ ⎞ ⎛ gn ∂n ⎞ ⎪ ⎟⎟ ⎬ Δp ⎜⎜ log ⎢ ⎥ + g log ⎢ ⎥ ⎟⎟ ⎜⎜ + ⎪ ∂p ⎠ ⎭ ⎣ Jn ⎦ ⎣ pn ⎦ ⎠ ⎝ p ⎝ ⎧ ⎫ ⎪ Δp ⎪ ⎬ dΩ 0 = R f + ρf Jk ⎨ ∇x (δp). ∇x (Δp) + g ∇x (δp). ∇x p ⎪ p ⎪ ⎩ ⎭

Fig. 3. Typical finite element with nodal dofs in magneto-poromechanics.

(72)

306

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

where the first integral on the left-hand side corresponds to the fluid–solid coupling. Rf is the short hand notation for the residual of the fluid part. Finite element outlines In a finite element context, the displacement, the magnetic potential, and the pore pressure fields are defined at the nodes, see Fig. 3 for an illustration. The interpolations of the geometry and the three fields are completely standard, see e.g. Hughes (1987), Zienkiewicz and Taylor (2000), Wriggers (2008) for the exposition of these ideas. For the monolithic resolution, the element contributions to the global tangent stiffness matrix associated with the element nodes are written as

K eAB

⎡ K AB K AB K AB ⎤ e12 e13 ⎥ ⎢ e11 AB AB ⎢ = Ke 21 Ke 22 0 ⎥ ∈ (ndim + 2)×(ndim + 2) ⎥ ⎢ ⎥ ⎢⎣ KeAB 0 KeAB 31 33 ⎦

(73)

e e for A, B = 1, …nnode , where nnode is the number of nodes. In this matrix, the first column (row) is associated with the ndim components of the nodal displacements, the second column (row) is associated with the nodal magnetic potential, and the third column (row) is associated with the nodal fluid pore pressure. The fact that there is no coupling between magnetostatics and fluid mass conservation appears through the vanishing (2, 3) terms, i.e. KeAB = 0 and KeAB = 0. The expressions of 23 32 the different sub-matrices are easily deduced from the above linearizations, Eqs. (69), (70) and (72). In particular, the (1, 2) terms are symmetric, KeAB = (KeAB )T , but the (1, 3) ones are not. This renders the global tangent matrix non-symmetric. 21 12

5. Numerical simulations Since the solid skeleton is macroscopically compressible, it is beneficial to split the deformation locally into a volumetric part that depends on the Jacobian J, and an isochoric part that depends on the modified deformation gradient J−1/3 F , as originally proposed by Flory (1961), and successfully applied later on in finite strain elasticity, e.g. see Lubliner (1985), Ogden (1997), Simo and Hughes (1998), Holzapfel (2000) among many others. In practice, any of the existing compressible hyperelastic models proposed in the literature can be used for the effective drained response of the solid skeleton. We choose here a Neo-Hookean type with a free energy given by 3

1

′ (C ) = κsk (J4/3 + 2J−2/3 − 3) + μsk (J−2/3 C: 1 − 3) χsk 8 2

(74)

where the first term is related to the volumetric response with κsk as a bulk modulus, and the second term is related to the volume-preserving part of the response with μsk as a shear modulus. Hence, together with the expression already given for the porous space contribution, χpor (J , p) in Eq. (63), the augmented free energy (53) is completely defined. Of interest in this section is the qualitative modeling of macroporous ferrogels that can be used as active porous scaffolds capable of delivering biological agents under the controls of external magnetic stimuli. Various macroporous ferrogels were developed and studied in Zhao et al. (2011). In particular, we consider here the one fabricated with 13 wt % Fe3O4 and 1 wt % alginate cross-linked by 5 mM AAD (adipic acid dihydrazide), and frozen at 20 °C. It is characterized by its highly

Fig. 4. Compression tests on the macroporous ferrogel. Fast loading/unloading at 0.85 s−1 (solid curve), and very slow loading/unloading (dashed curve). Finite element mesh and selected deformed configurations at 50% and 85% compressive strains.

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

307

interconnected (initial) porosity, about 82%, and a low initial modulus, about 2.5 kPa. We keep in mind these two important informations for the following simulations. 5.1. Response to mechanical loadings Fig. 4 shows the results of compression tests on a cylindrical sample of radius 5 mm and 15 mm height. The lateral free surface is supposed to allow drainage while the top and bottom faces are assumed smooth and impervious. The initial pore pressure is set to p0 = 1 atm , this latter being the prescribed value of the pore pressure on the lateral surface as a boundary condition for the fluid part. The mechanical loading consists on imposing a displacement on the top face while the bottom one remains fixed. For symmetry reasons, one fourth of the cylinder is considered during the computations. The following poromechanics material parameters have been used:

κsk = 0.83334 kPa, f0 = 0.82,

μsk = 1.25 kPa,

m = 1.2,

k 0 = 100 mm2 /MPa s,

Q = 500 kPa, ρ f0 = 1.204 kg/m3,

g=1

(75)

where κsk and μsk are such that Young's modulus is E0 = 2.5 kPa in the limiting case of a linearized kinematics with a zero Poisson's ratio, i.e. the macroporous ferrogel behaves like a sponge, see also Hong et al. (2014). Besides on the known initial porosity f0, see above, the parameters Q and m are only qualitative. Nevertheless, these (f0 , m , Q ) parameters together with p0 = 1 atm are the ones with which the porosity law of Fig. 2 has been plotted. For the fluid constitutive law, see Eq. (68), the fluid parameter g corresponds to an ideal gas, ρ f0 being here the initial air density. Finally, the material permeability coefficient k0 is also qualitative at this stage. Anyhow, this latter influences the rate-effects of the sample's response through Darcy's law. This is shown by comparing the two loading/unloading curves of Fig. 4. The dashed one corresponds to the case of a very slow velocity with full drainage, i.e. the effective hyperelastic response of the solid skeleton alone. The solid curve corresponds to a faster velocity where the sample is strain compressed at 85% in one second of time. A relative stiffening is observed in this case with the characteristic hysteresis due to the delay caused by the fluid flow during unloading. Globally, these results are in good agreement with the ones obtained experimentally in Zhao et al. (2011). The high deformability of the macroporous ferrogel is well captured by the purely poromechanical part of the present modeling framework. 5.2. Macroporous ferrogel under magnetic loading In this second step, the deformation of macroporous ferrogel under the influence of a magnetic field is examined. The sample we consider is again the above cylinder with the same compressible Neo-Hookean-like material. For the magnetic field, we recall that μ0 = 4π10−7 N/A2 for the magnetic permeability of vacuum. The magnetization parameters c1, c2 and c3, see Eq. (53), would have to be determined experimentally. However, due to the lack of experimental results, material

a

b

Fig. 5. Deformed configuration under: (a) Δφ = 1 A and (b) Δφ = 2 A .

308

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

Fig. 6. Evolution of the compressive strain with the magnetic loading. Deformed configurations for Δφ = 0.6 and 2 A during loading, and Δφ = 0.1 A during unloading.

properties are inadequate at this point. Therefore, for the purpose of testing the robustness of our numerical implementation, we assume the following values in this example:

c1 = 1 N/A2,

c2 = 1 N/A2,

c3 = 1 N/A2

(76)

to activate the three pseudo-invariants relative to the magnetic coupling in the constitutive relations, see the expressions (54), or (56), for the stress tensor, and (58), or (59), for the magnetic induction vector. A magnetic potential φ is imposed on the two ends of the cylinder at φ and φ þ , respectively, which create a potential difference Δφ = φ+ − φ−. During the computation, this difference is increased from 0 to 2 A in 20 steps at a loading velocity of 0.5 A/s, and then decreased from 2 to 0 A in 20 steps as well at an unloading velocity of 0.5 A/s. For the rest of the boundary conditions, the two end faces are free and impervious, and the lateral surface is free with a prescribed pore pressure set to p0 for the fluid part. This latter is also the initial pore pressure in the whole cylinder before the magnetic loading. The deformation of the cylinder is shown in Fig. 5 for the magnetic potential differences Δφ = 1 A and Δφ = 2 A during the loading phase. For illustrative purposes, the Eulerian porosity distribution for the latter and the pore pressure field for the former are also shown. Among others, these fields are not uniform within the cylinder and, due to the relatively high permeability of the porous space together with the small dimensions of the sample, the difference of the pore pressure with the initial one, p0 = 105 N/m2, is small. One can also observe that the deformation easily reaches large levels, more than 70%. This is highlighted in Fig. 6 where we have plotted the evolution of the global compressive strain versus the magnetic loading. The hysteresis that appears during unloading illustrates here again the rate-effects due to the fluid-flow.

Fig. 7. Evolution of the released volume of water from the whole domain under a one-cycle (dashed curve) and three-cycles (solid curve) magnetic loading histories. The computations are pursued until almost total recovery.

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

309

5.3. Macroporous ferrogels as active sponges Macroporous ferrogels can be used as devices in tissue engineering and cell-based therapies to trigger and enhance the release of various biological agents by controlling the external magnetic fields, see Zhao et al. (2011) for more details. It becomes then of major importance to know how the amount of released fluid evolves during the loading history. Within the present theory, this information is provided by the fluid mass conservation equation, i.e. by Eq. (6), or equivalently by Eq. (65)3. As an example, we consider again the precedent macroporous cylindrical sample of radius 5 mm and 15 mm height. This latter is this time completely submerged in water. The magneto-poromechanics material parameters we use are those given in Eqs. (75) and (76) less those for the fluid's constitutive law, replaced here by

ρ f0 = 1000 kg/m3 and

g=0

for the saturating incompressible water. Initially, the volume of water inside the porous domain is then ∼966.04 mm3 in our case, i.e. the initial volume of the cylinder times the initial porosity f0. Now as for the example of Section 5.2, a loading/unloading cycle consists of an increase of the potential difference Δφ between the end faces from 0 to 2 A at a velocity of 0.5 A/s, followed by a decrease from 2 A to 0 A at a velocity of 0.5 A/s. The boundary conditions are the same as for the precedent example. For illustrative purposes, Fig. 7 shows the evolution of the released water volume from the whole cylinder under a one-cycle and three-cycles magnetic loading histories. Noteworthy observations should be pointed out from these results:

While the ascending branches of the curves correspond to increasing volume release when the magnetic loading is

increasing, the descending ones mean that the released water is being partially reabsorbed with decreasing magnetic loading. Once the magnetic loading is off, almost all the released water is reabsorbed after a recovery time and the cylindrical sample returns to its original underformed configuration. One can check that, at any time, the computed released volume of water never exceeds the volume that was initially present inside the sample, i.e. less than ∼966.04 mm3.

6. Conclusion and perspectives In this paper, we have presented a coupled magneto-poromechanics theory where, for the poromechanics part, use has been made of the macroscale Biot's theory. By means of the continuum thermodynamics of open media, the nowadays well known fields related to the magnetic coupling have been embedded in a sound way for a concise characterization of the whole set of constitutive equations. Furthermore, as large deformation is usually expected due to the soft nature of the materials we have in mind, the present theory has been developed within the finite strain range. To make matters as concrete as possible, a magneto-hyperelastic model has been presented in detail that can be well adapted for the modeling of macroporous ferrogels. As these latter can further give high porosity change, a nonlinear porosity law has been used that allows for a good description of the seepage process when the fluid is released and/or reabsorbed. This characteristic can certainly be of particular interest for the design of biomedical devices used to enhance the release of biological agents. With the finite element method as a tool for structural simulations, the numerical examples presented in this paper have shown an encouragingly good agreement with experimental observations, at least qualitatively. We believe that further work has to be accomplished to optimize the present formulation toward more realistic modeling of smart magneto-active porous materials in general. Experimental investigations will certainly give better knowledge of the material properties. Among others, the correct evaluation of the fluid permeability which, even high and allows rapid recovery, has however a great importance on the seepage process and, consequently, on the rate-depend effects due to the fluid flow. The magnetization parameters c1, c2 and c3 must be quantified correctly. Experimental tests could for example show which ones are most relevant for the modeling, so that the coupling part of the constitutive relations could then be simplified. Further algorithmic investigations in conjunction with optimized finite elements are needed. This is especially true for problems where strong distorsions at large deformations with highly compressible materials are present. The present global resolution strategy using a simultaneous scheme must be changed in the favor of a straggered scheme exploiting the symmetries of each sub-problem with certainly less computational costs. Moreover, as Maxwell equations must be satisfied not only inside the body, but also in the surrounding free space, this fact must be accounted for in future numerical developments. On another hand, when dealing with problems in magnetodynamics, a vector potential formulation must be used together with the magnetic induction vector as main magnetic variable. These points and others will form the substance of separate communications.

310

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

Appendix A. Fluid mass conservation within a porous material Within any volume

df dt

∫Ω

t

Ωt of porous material in the spatial configuration, the Eulerian fluid mass conservation is given by

ρf n dΩt = 0

(A.1)

where n is the Eulerian porosity and

ρf is the current fluid density. Eq. (A.1) leads to the following local form:

∂ (ρ n) + div (ρf nvf ) = 0 ∂t f

(A.2)

where vf is the velocity of the fluid phase located at x . Now as the spatial flux vector of fluid mass qf is given by, see Fig. 1,

qf = ρf n (vf − vs )

(A.3)

where vs is the velocity of the solid phase at the same location x , Eq. (A.2) is equivalently rewritten as

ds (ρ n) + ρf n div vs + div qf = 0 dt f

(A.4)

in terms of the material time derivative with respect to the solid phase. Integrating the last result over the actual volume Ωt gives

ds dt

∫Ω

t

ρf n dΩt +

∫Ω

t

div qf dΩt = 0

(A.5)

which proves the identity of Eq. (3).

Appendix B. Thermostatics of fluids Let us recall basic relations on the thermostatics of fluids that are useful in the continuum thermodynamic developments of Section 3, see for example Coussy (2004) for more details. The energy conservation reads

⎛ 1⎞ def = − pd ⎜⎜ ⎟⎟ + δQ ⎝ ρf ⎠

(B.1)

where def is the change of the specific internal energy of the fluid, δQ is the infinitesimal heat supply, and −pd (1/ρf ) is the mechanical work supplied to the fluid by the pressure p in the volume change d (1/ρf ) of its specific volume 1/ρf . Excluding irreversible transformations, the entropy balance reads

dsf =

δQ T

(B.2)

where sf is the specific entropy of the fluid and T the absolute temperature. Combination of Eqs. (B.1) and (B.2) by eliminating the heat supply leads to the following energy balance:

⎛ 1⎞ def = − pd ⎜⎜ ⎟⎟ + Tdsf ⎝ ρf ⎠

(B.3)

This latter means that the specific internal energy has arguments 1/ρf and sf, i.e. ef ≡ ef (1/ρf , sf ). By identification, again with Eq. (B.3), we get the state laws

p= −

∂ef ⎛ 1⎞ ∂ ⎜⎜ ⎟⎟ ⎝ ρf ⎠

and

T=

∂ef ∂sf (B.4)

Partial inversion with respect to the pair (1/ρf , p) gives the fluid specific enthalpy hf as 1 p hf ≡ hf (p, sf ) = ef − ( )( − p) = ef + ρf ρf

(B.5)

Hence, the variation of this latter, and use of Eq. (B.3), identify the state laws

∂hf 1 = ρf ∂p

and

T=

∂hf ∂sf

(B.6)

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

311

Partial inversion, this time with respect to the pair (sf , T ), gives the fluid specific free energy ψf as ⎛1 ψf ≡ ψf ⎜⎜ , ⎝ ρf

⎞ T ⎟⎟ = ef − Tsf ⎠

(B.7)

Its variation together with the use of Eq. (B.3), identify the state laws

p= −

∂ψf ⎛ 1⎞ ∂ ⎜⎜ ⎟⎟ ⎝ ρf ⎠

sf = −

and

∂ψf ∂T (B.8)

Finally, total inversion with respect to both pairs gives the fluid specific free enthalpy μf, i.e. the Gibbs specific potential, as μf ≡ μf (p, T ) = ef +

p − Tsf ρf

(B.9)

with the state laws

∂μf 1 = ρf ∂p

and

sf = −

∂μf ∂T

(B.10)

∼ Appendix C. Augmented tangent modulus C ∼ As for the augmented stress tensor, Eqs. (54) or (56), the fourth-order tangent modulus C is given by an additive form as well. We write ∼ C = Csk + Cpor + Cmgn (C.1) where Csk is the modulus relative to the drained hyperelastic solid skeleton, Cpor is the porous space contribution at fixed pore pressure, and Cmgn is the magnetic contribution at fixed magnetic potential due to both the magneto-mechanics coupling and the magnetic augmentation. The derivation of Csk mimics those for single-phase hyperelastic solids widely developed in the literature, see e.g. Ogden (1997), Simo (1998), Holzapfel (2000), Nedjar (2002a,b, 2011), Wriggers (2008). Details of this nowadays standard notion are skipped here. For the derivation of the modulus Cpor , one proceeds in two steps starting from the definition of the partial state law Spor = Jσpor C −1, Eq. (55)2, on the reference configuration where we have defined the (scalar) volumetric Cauchy stress σpor = ∂χpor /∂J : ̇ = Ξpor : 1 Ċ , where Ξpor is the material tangent modulus relative to the step (i): compute the time derivative such that Spor 2 porous space; step (ii): then, push-forward of the precedent result to the current configuration with the solid skeleton's deformation ̇ FT such that £v τpor = Cpor : d , where d = sym [FF ̇ −1] is the spatial strain rates gradient F gives the Lie derivative £v τpor ≡ FSpor ̇ tensor. The useful kinematic relationship C = 2FT dF is to be employed during the derivation, see Nedjar (2002, 2007, 2011) for similar developments. The following expression is then obtained

⎧ ∂σpor ⎫ ⎬1 ⊗ 1 Cpor = − 2Jσpor I + J ⎨ σpor + J ⎩ ∂J ⎭

(C.2)

The derivation of the modulus Cmgn follows similar lines as for Cpor , this time starting from the partial stress

S mgn = 2c2 ⊗ + 2c3 { ⊗ C + C ⊗ } 1

− 2 μ 0 J (C −1: ⊗ ) C −1 + μ 0 JC −1 ⊗ C −1

(C.3)

̇ FT , allows to identify i.e. the last four terms in Eq. (54). Push-forward of its time derivative to the current configuration, FSmgn the following partial tangent modulus:

Cmgn = 4c3 Ib − 2μ 0 I 1

+ μ 0 J (. ){I − 2 1 ⊗ 1 + 1 ⊗ ⊗ + ⊗ ⊗ 1}

(C.4)

where the fourth-order operators I and Ib are defined such that

I: A = ⊗ A + A ⊗ Ib: A = b ⊗ bAb + bAb ⊗ b for any second order tensor A .

(C.5)

312

B. Nedjar / J. Mech. Phys. Solids 84 (2015) 293–312

References Armero, F., 1999. Formulation and finite element implementation of a multiplicative model of coupled poro-plasticity at finite strains under fully saturated conditions. Comput. Methods Appl. Mech. Eng. 171, 205–241. Baek, S., Pence, T., 2011. Inhomogeneous deformation of elastomer gels in equilibrium under saturated and unsaturated conditions. J. Mech. Phys. Solids 59, 561–582. Biot, M., 1941. General theory of three-dimensional consolidation. J. Appl. Phys. 12, 155–164. Biot, M., 1972. Theory of finite deformation of porous solids. Indiana Univ. Math. J. 21, 597–620. Bowen, R., 1982. Compressible porous media models by use of the theory of mixtures. Int. J. Eng. Sci. 20, 697–735. Brigadnov, I., Dorfmann, A., 2003. Mathematical modeling of magneto-sensitive elastomers. Int. J. Solids Struct. 40, 4659–4674. Brown, W., 1966. Magnetoelastic Interactions. Springer, Berlin. Bustamante, R., Dorfmann, A., Ogden, R., 2006. Universal relations in isotropic nonlinear magnetoelasticity. Q. J. Mech. Appl. Math. 59, 435–450. Bustamante, R., Dorfmann, A., Ogden, R., 2008. On variational formulations in nonlinear magnetoelastostatics. Math. Mech. Solids 13, 725–745. Chadwick, P., 1976. Continuum Mechanics. Concise Theory and Problems. John Wiley and Sons, Inc., New York, NY. Coleman, B., Gurtin, M., 1967. Thermodynamics with internal variables. J. Chem. Phys. 47, 597–613. Coussy, O., 2004. Poromechanics. John Wiley and Sons Inc., New York. Dorfmann, A., Ogden, R., 2004a. Nonlinear magnetoelastic deformations. Q. J. Mech. Appl. Math. 57, 599–622. Dorfmann, A., Ogden, R., 2004b. Nonlinear magnetoelastic deformations of elastomers. Acta Mech. 167 (1–2), 13–28. Duda, F., Souza, A., Fried, E., 2010. A theory for species migration in a finitely strained solid with application to polymer network swelling. J. Mech. Phys. Solids 58, 515–529. Ericksen, J., 2006. A modified theory of magnetic effects in elastic materials. Math. Mech. Solids 11, 23–47. Flory, P., 1961. Thermodynamic relations for high elastic materials. Trans. Faraday Soc. 57, 829–838. Germain, P., Nguyen, Q., Suquet, P., 1983. Continuum thermodynamics. ASME J. Appl. Mech. 50, 1010–1021. Ginder, J., Clark, S., Schlotter, W., Nichols, M., 2002. Magnetostrictive phenomena in magnetorheological elastomers. Int. J. Mod. Phys. B 16, 2412–2418. Holzapfel, G., 2000. Nonlinear Solid Mechanics. A Continuum Approach for Engineering. John Wiley and Sons, Ltd, Chichester, West Sussex, UK. Hong, S., Jung, Y., Yen, R., Chan, H., Leong, K., Truskey, G., Zhao, X., 2014. Magnetoactive sponges for dynamic control of microfluidic flow patterns in microphysiological systems. Lab Chip 14, 514–521. Hughes, T., 1987. The Finite Element Method. Prentice-Hall, Englewood-Cliffs, NJ. Jolly, M., Carlson, J., Muñoz, B., 1996. A model of the behavior of magnetorheological materials. Smart Mater. Struct. 5, 607–614. Kankanala, S., Triantafyllidis, N., 2004. On finitely strained magnetorheological elastomers. J. Mech. Phys. Solids 52, 2869–2908. Kovetz, A., 2000. Electromagnetic Theory. Oxford University Press, Oxford. Lewis, R., Schrefler, B., 1998. The Finite Element Method in the Static and Dynamic Deformation and Consolidation of Porous Media. John Wiley and Sons Inc., New York. Liu, T., Hu, S., Liu, K., Liu, D., Chen, S., 2006. Preparation and characterization of smart magnetic hydrogels and its use for drug release. J. Magn. Magn. Mater. 304, e397–e399. Lubliner, J., 1985. A model of rubber viscoelasticity. Mech. Res. Commun. 12, 93–99. Marsden, J., Hughes, T., 1983. Mathematical Foundations of Elasticity. Prentice-Hall, Englewood-Cliffs, NJ. Nedjar, B., 2002. A theoretical and computational setting for a geometrically nonlinear gradient damage modelling framework. Comput. Mech. 30, 65–80. Nedjar, B., 2002a. Frameworks for finite strain viscoelastic-plasticity based on multiplicative decompositions. Part I: continuum formulations. Comput. Methods Appl. Mech. Eng. 191, 1541–1562. Nedjar, B., 2002b. Frameworks for finite strain viscoelastic-plasticity based on multiplicative decompositions. Part II: computational aspects. Comput. Methods Appl. Mech. Eng. 191, 1563–1593. Nedjar, B., 2007. An anisotropic viscoelastic fibre-matrix model at finite strains: continuum formulation and computational aspects. Comput. Methods Appl. Mech. Eng. 196 (9–12), 1745–1756. Nedjar, B., 2011. On a continuum thermodynamics formulation and computational aspects of finite growth in soft tissues. Int. J. Numer. Methods Biomed. Eng. 27, 1850–1866. Nedjar, B., 2013a. Formulation of a nonlinear porosity law for fully saturated porous media at finite strains. J. Mech. Phys. Solids 61 (2), 537–556. Nedjar, B., 2013b. Poromechanics approach for modeling closed-cell porous materials with soft matrices. Int. J. Solids Struct. 50, 3184–3189. Nedjar, B., 2014. On finite strain poroplasticity with reversible and irreversible porosity laws. Formulation and computational aspects. Mech. Mater. 68, 237–252. Ogden, R., 1997. Non-linear Elastic Deformations. Dover, New York. Pao, Y., 1978. Electromechanic forces in deformable continua. In: Nemat-Nasser, S. (Ed.), Mechanics Today, vol. 4. . Oxford University Press, Oxford, pp. 209–305. Simo, J., 1998. Numerical analysis and simulation of plasticity. In: Ciarlet, P., Lions, J. (Eds.), Handbook of Numerical Analysis, vol. VI. . North-Holland, Amsterdam, pp. 183–499. Simo, J., Hughes, T., 1998. Computational Inelasticity. Springer-Verlag, New York. Spencer, A., 1984. Constitutive theory for strongly anisotropic solids. In: Spencer, A. (Ed.), Continuum Theory of the Mechanics of Fibre-reinforced Composites. CISM Cources and Lectures No. 282. Springer, Wien. Steigmann, D., 2004. Equilibrium theory for magnetic elastomers and magnetoelastic membranes. Int. J. Non-Linear Mech. 39, 1193–1216. Truesdell, C., Noll, W., 1965. The nonlinear field theories of mechanics. In: Fluegge, S. (Ed.), Handbuch der Physik Bd. III/3. Springer-Verlag, Berlin. Varga, Z., Filipcsei, G., Zrínyi, M., 2006. Magnetic field sensitive functional elastomers with tunable elastic modulus. Polymer 47, 227–233. Vu, D., Steinmann, P., 2007. Nonlinear electro- and magneto-elastostatics: material and spatial settings. Int. J. Solids Struct. 44, 7891–7901. Wilmanski, K., 2003. On thermodynamics of nonlinear poroelastic materials. J. Elast. 71, 247–261. Wriggers, P., 2008. Nonlinear Finite Element Methods. Springer-Verlag, Berlin, Heidelberg. Zhao, X., Kim, J., Cezar, C., Huebsch, N., Lee, K., Bouhadir, K., Mooney, D., 2011. Active scaffolds for on-demand drug and cell delivery. Proc. Natl. Acad. Sci. 108 (1), 67–72. Zienkiewicz, O., Taylor, R., 2000. The Finite Element Method, 5th ed., vol. 1. Butterworth-Heinemann, Oxford, UK. Zrínyi, M., Barsi, L., Büki, A., 1996. Deformation of ferrogels induced by nonuniform magnetic fields. J. Chem. Phys. 104 (21), 8750–8756.

Copyright © 2020 COEK.INFO. All rights reserved.